NANOMATERIALS Atomically thin two-dimensional organic ... · Organic-inorganic hybrid perovskites,...
Embed Size (px)
Transcript of NANOMATERIALS Atomically thin two-dimensional organic ... · Organic-inorganic hybrid perovskites,...
Matter MURI, NIST, and NSF (through the Physics Frontier Centerat the JQI). B.K.S. is a NIST–National Research CouncilPostdoctoral Research Associate. L.M.A. was supported by theNSF Graduate Research Fellowship Program. All authors exceptI.B.S contributed to the data collection effort. B.K.S. and L.M.A.configured the apparatus for this experiment. H.-I.L. led theteam on all aspects of the edge-current and skipping-orbitmeasurements. H.-I.L., L.M.A., and B.K.S. analyzed data. B.K.S.,
H.-I.L., L.M.A, and I.B.S. performed numerical and analyticalcalculations. All authors contributed to writing the manuscript.I.B.S. proposed the initial experiment.
www.sciencemag.org/content/349/6255/1514/suppl/DC1Materials and Methods
Supplementary TextFig. S1Reference (35)Database S1
9 February 2015; accepted 28 July 201510.1126/science.aaa8515
Atomically thin two-dimensionalorganic-inorganic hybrid perovskitesLetian Dou,1,2* Andrew B. Wong,1,2* Yi Yu,1,2,3* Minliang Lai,1 Nikolay Kornienko,1,2
Samuel W. Eaton,1 Anthony Fu,1,2 Connor G. Bischak,1 Jie Ma,2 Tina Ding,1,2
Naomi S. Ginsberg,1,2,4,5,6 Lin-Wang Wang,2 A. Paul Alivisatos,1,2,5,7 Peidong Yang1,2,5,7†
Organic-inorganic hybrid perovskites, which have proved to be promising semiconductormaterials for photovoltaic applications, have been made into atomically thin two-dimensional(2D) sheets.We report the solution-phase growth of single- and few-unit-cell-thicksingle-crystalline 2D hybrid perovskites of (C4H9NH3)2PbBr4 with well-defined squareshape and large size. In contrast to other 2D materials, the hybrid perovskite sheetsexhibit an unusual structural relaxation, and this structural change leads to a band gapshift as compared to the bulk crystal.The high-quality 2D crystals exhibit efficientphotoluminescence, and color tuning could be achieved by changing sheet thickness aswell as composition via the synthesis of related materials.
The organic-inorganic hybrid perovskites,especially CH3NH3PbI3, have recently beenused in solution-processable photovol-taic devices that have reached 20% powerconversion efficiency (1–4). These layered
materials have a general formula of (RNH3)2(CH3NH3)m-1AmX3m+1, where R is an alkyl oraromatic moiety, A is a metal cation, and X isa halide. The variable m indicates the numberof the metal cation layers between the two lay-ers of the organic chains (5–11). In the extremecase where m = V, the structure becomes athree-dimensionally bonded perovskite crystalwith a structure similar to BaTiO3. In the oppo-site extreme wherem = 1, the structure becomesan ideal quantum well with only one atomiclayer of AX4
2– separated by organic chains, inwhich the adjacent layers are held together byweak van der Waals forces.This arrangement is fundamentally different
from transition metal dichalcogenides, in whichone layer of the metal ions is sandwiched be-tween two hexagonal layers of S or Se atoms,affording a rigid backbone. In contrast, the lay-
ered hybrid perovskites normally have a tetrago-nal or orthorhombic structure and are inherentlymore flexible and deformable (5–11). By varyingthe value of m, the thickness and the relatedoptoelectronic properties of the quantum wellcan be tuned. To date, many organic amines,metal cations (Cu2+, Mn2+, Cd2+, Ge2+, Sn2+, Pb2+,Eu2+, etc.) and halides (Cl, Br, and I) have beenused to construct such layered materials (m =1 ~ 3), and their corresponding optoelectronicproperties have been well studied (12–15). Pre-vious reports have claimed that the organic layerseffectively isolate the two-dimensional (2D) quan-tum wells in each layer from electronic coupling,if the organic chain is longer than propyl amine(16). This means that the properties of the atomi-cally thin 2D quantum well should be the sameas those of the bulk layered material (microscopiccrystal, powder, or film). This hypothesis, as wellas the technical difficulty of separating individuallayers, has probably delayed investigation of free-standing single layers of such 2D materials. Veryrecently, attempts to obtain ultrathin 2D perov-skite samples by spin coating, chemical vapor de-position, or mechanical exfoliation methods havebeen made with limited success (17–19).Here we report the direct growth of atomically
thin 2D hybrid perovskites [(C4H9NH3)2PbBr4]and derivatives from solution. Uniform square-shaped 2D crystals on a flat substrate with highyield and excellent reproducibility were syn-thesized by using a ternary co-solvent. We in-vestigated the structure and composition ofindividual 2D crystals using transmission elec-tron microscopy (TEM), energy-dispersive spec-
troscopy (EDS), grazing-incidence wide-anglex-ray scattering (GIWAXS), and Raman spec-troscopy. Unlike other 2D materials, a struc-tural relaxation (or lattice constant expansion)occurred in the hybrid perovskite 2D sheetsthat could be responsible for emergent features.We investigated the optical properties of the 2Dsheets using steady-state and time-resolved pho-toluminescence (PL) spectroscopy and cathodolu-minescence microscopy. The 2D hybrid perovskitesheets have a slightly shifted band edge emissionthat could be attributed to the structural relaxa-tion. We further demonstrated that the as-grown2D sheets exhibit high PL quantum efficiency aswell as wide composition and color tunability.A structural illustration of a monolayer 2D
perovskite (Fig. 1A) shows the case with six Bratoms surrounding each Pb atom, and the fourin-plane Br atoms are shared by two octahedrons,forming a 2D sheet of PbBr4
2–. The negativecharges are compensated for by the butylam-monium that caps the surfaces of the 2D sheet.This structure is amenable to facile solution syn-thesis. The ionic character of such materials isstronger than the transition metal disulfidesand diselenides, and the bulk solid is soluble inpolar organic solvents such as dimethylformamide(DMF) (20). To grow 2D sheets, a very dilute pre-cursor solution was dropped on the surface of aSi/SiO2 substrate and dried under mild heating[see the supplementary materials (21)]. A DMFand chlorobenzene (CB) co-solvent was initiallyinvestigated, because CB helps to reduce the sol-ubility of (C4H9NH3)2PbBr4 in DMF and pro-mote crystallization. Because CB has a similarboiling point and evaporation rate as DMF, thedrying of the solvents and the crystallizationprocess were uniform across the whole substrate.We examined the products of this reaction by
optical microscopy and atomic force microscopy(AFM), but instead of monolayers, thick par-ticles with random shapes formed on the sub-strate (fig. S1). Hybrid perovskites have limitedsolubility in acetonitrile, and the solvent hasbeen used previously for making microscopichybrid perovskite single crystals (22). In thiscase, acetonitrile evaporates more quickly andhelps induce the formation of the ultrathin 2Dhybrid perovskite sheets. When acetonitrile wascombined with DMF and CB, uniform squaresheets grew on the substrate (Fig. 1B). The edgelength of the square crystals ranged from 1 to10 mm, with an average of 4.2 mm (the size dis-tribution statistics can be found in fig. S2). Thedetailed synthetic procedure and discussion ofthe role of each solvent can be found in the sup-plementary text (21).
1518 25 SEPTEMBER 2015 • VOL 349 ISSUE 6255 sciencemag.org SCIENCE
1Department of Chemistry, University of California, Berkeley, CA94720, USA. 2Materials Sciences Division, Lawrence BerkeleyNational Laboratory, Berkeley, CA 94720, USA. 3School ofPhysical Science and Technology, ShanghaiTech University,Shanghai, 201210, China. 4Department of Physics, University ofCalifornia, Berkeley, CA 94720, USA. 5Kavli Energy NanoScienceInstitute, Berkeley, CA 94720, USA. 6Physical Biosciences Division,Lawrence Berkeley National Laboratory, Berkeley, CA 94720, USA.7Department of Materials Science and Engineering, University ofCalifornia, Berkeley, CA 94720, USA.*These authors contributed equally to this work. †Correspondingauthor. E-mail: [email protected]
RESEARCH | REPORTSon M
ay 28, 2020
The thickness of the square sheets was quan-tified with AFM. The thickness of the crystalsvaried from a few to tens of nanometers; thethinnest sheets were ~1.6 nm (±0.2 nm). TheAFM images of several monolayer and double-layer sheets show thicknesses of 1.6 and 3.4 nm(±0.2 nm) (Fig. 1, C and D), whereas the dspacing in the bulk crystal was 1.4 nm (20).AFM tapping mode (noncontact) was used toavoid sample damage, which can lead to a minoroverestimation. For the separated monolayer, theorganic chain may also relax, and the apparentthickness of the monolayer may increase slight-ly. Additional AFM images of other similar 2Dsheets can be seen in fig. S3.By combining AFM and optical microscopy,
we correlated the appearance of the sheets inthe optical image with their thickness as shownin fig. S4. The thinnest sheet on Si/SiO2 that wecould distinguish in an optical microscope wasa double layer. We also prepared large single
crystals of (C4H9NH3)2PbBr4 and investigatedthe conventional mechanical exfoliation methodusing tape and the solvent exfoliation methodusing hexane to disperse the thin sheets (23).Unfortunately, the majority of the products frommechanical exfoliation were very thick flakes (fig.S5A) and from solvent exfoliation they were ran-domly shaped particles (fig. S5, B and C). Themonolayer-thick particles obtained were verysmall (less than 1 mm), which suggests that thesehybrid perovskite layers are mechanically brittle.To determine the crystal structure of the 2D
hybrid perovskites, x-ray diffraction (XRD) andTEM were used. The XRD pattern revealed thatthe (001) plane grew parallel to the substrate,and the out-of-plane d spacing was 1.42 nm (fig.S6), which is consistent with reported data forthis material (16). The in-plane structural infor-mation was revealed by selected-area electrondiffraction (SAED) in a TEM. Figure 2A shows aTEM image of a 2D sheet grown on a lacy car-
bon grid. After examining more than 20 indi-vidual sheets by TEM, we found that they allshowed similar shape and identical diffractionpatterns (additional TEM images are shown fig.S7); Fig. 2B shows the SAED pattern of anothersheet. The calculated average in-plane latticeconstants are a = 8.41 Å and b = 8.60 Å from fivesheets, which are slightly greater than the latticeconstants in the bulk crystal measured by single-crystal XRD [a = 8.22 Å and b = 8.33 Å, see (15)and tables S1 and S2]. The electron diffractionpatterns were consistent with structural simula-tions, which further confirm the structure of theatomically thin 2D sheets (see figs. S8 and S9 formore discussion on the simulations/experimentson the bulk and few-layer hybrid perovskites).We observed rapid radiation damage of the
sheets under the strong electron beam. Afterexposing the 2D sheets to the electron beam fora few seconds, Pb was reduced and precipitated,which caused the sample to be irreversibly dam-aged (fig. S10). This phenomenon is similar tothat observed in alkali halides (24). More exam-ples of SAED patterns of individual sheets andtheir corresponding TEM images demonstratingthe degradation can be found in fig. S11. Figure 2,C to F, shows the elemental distribution in thethin sheets; lead, bromine, carbon, and nitrogenare all present in the square.The lattice expansion in the 2D sheets was fur-
ther confirmed through macroscopic GIWAXSmeasurements. Figure 2G shows the GIWAXSimage and Fig. 2H shows the integrated pattern.In addition, to the (200) and (020) peaks ob-served in TEM diffraction, many other peaks canbe assigned. The d spacing of the (200), (020), (111),and (113) planes is 4.19 (lattice constanta=8.38 Å),4.25 (lattice constant b = 8.50 Å), 5.81, and 5.00 Å;respectively. These values are all greater thanthose of the bulk crystals and are consistentwith our TEMmeasurements of single 2D sheets.In addition, we examined the Raman spectra
of the bulk crystal and the thin sheet as shownin fig. S12. The peaks found at 57.7 and 43.6 cm−1
for the bulk crystal shifted to 55.2 and 41.3 cm−1
for the 2D sheet, respectively. These peaks can beattributed to Pb-Br stretching and librationalmotions of both inorganic and organic ions (25),indicating that relaxation of the crystal latticeoccurs in the thin sheets. Meanwhile, the peakat 122.2 cm−1 (from -CH3 group torsional mo-tion and insensitive to lattice distortion) didnot change. The peaks for the 2D sheet becamenarrower, suggesting better-defined vibrationalstates in the thin sheet. Furthermore, our densityfunctional theory (DFT) calculation indicates asmall lattice expansion of around 0.1 Å for the mono-layer as compared to the bulk (C4H9NH3)2PbBr4crystal (see the supplementary materials for de-tails about DFT simulation).Strong crystal lattice distortions are common
for hybrid perovskites (5–10). Structural distortion–induced optical and electronic changes havebeen reported in bulk hybrid perovskites (26–29).Single-crystal XRD data of the bulk crystal of(C4H9NH3)2PbBr4 revealed that the PbBr4
2– layerin the bulk crystal is highly distorted, with a
SCIENCE sciencemag.org 25 SEPTEMBER 2015 • VOL 349 ISSUE 6255 1519
Fig. 1. Synthesis of atomically thin 2D (C4H9NH3)2PbBr4 crystals. (A) Structural illustration of asingle layer (C4H9NH3)2PbBr4 (blue balls, lead atoms; large orange balls, bromine atoms; red balls,nitrogen atoms; small orange balls, carbon atoms; H atoms were removed for clarity). (B) Opticalimage of the 2D square sheets. Scale bar, 10 mm. (C) AFM image and height profile of several singlelayers. The thickness is around 1.6 nm (T0.2 nm). (D) AFM image and height profile of a double layer.The thickness is around 3.4 nm (T0.2 nm).
RESEARCH | REPORTSon M
ay 28, 2020
Pb-Br-Pb bond angle of 152.94° (see fig. S13 andtables S3 and S4 for more details), which mayprovide driving forces for lattice relaxation inthe 2D thin sheet. In other reported 2D mate-rials, the in-plane crystal structure does notchange from the bulk crystal to isolated sheets;and the optical and electronic properties changebecause of electronic decoupling between adja-cent layers.We investigated the PL properties of indi-
vidual 2D crystals under 325-nm laser excitation.Figure 3A shows the PL spectra of the bulk(C4H9NH3)2PbBr4 crystal and 2D sheets withdifferent thickness (22, 8, and 3 layers thick, seefig. S14 for AFM images), and Fig. 3, B to E, showsthe corresponding PL image of each sheet. Boththe bulk materials and the sheets exhibit similarstrongpurple-blue light emission. The bulk crystalhas an emission peak at 411 nm (2.97 eV), and the2D sheets have slightly blue-shifted peaks at~406 nm (3.01 eV). The slightly increased opticalband gap for the ultrathin 2D sheets is probablyinduced by the lattice expansion. Our DFT sim-ulation also suggests a 20-meV blue shift in PLfor the single-layer 2D sheets, which is a trendconsistent with the experimental observation.The 2D sheets with different thickness (from 22to 3 layers) have similar PL spectra, the peak po-sition shift is within 1 nm, and any lattice con-stant difference is within the experimental errorfrom SAED observed between these samples.More discussion about the PL can be found inthe supplementary text (21).Cathodoluminescence microscopy, a technique
that provides a map of the light emitted from a
sample when excited by a focused electron beamwith excellent lateral resolution, was used to de-termine the spatial distribution of emissive siteson the 2D sheets. As shown in Fig. 3G, the cath-odoluminescence mapping from 395 to 435 nmshows a square shape identical to the correspond-ing scanning electron microscopy (SEM) imagesas shown in Fig. 3F, indicating that the emission isfrom the whole square. The PL internal quantumefficiency (QE) of the 2D sheets was estimated bycomparing the integrated PL intensity (from 390to 450 nm) of the band edge emission at roomtemperature (298 K) and helium cryogenic tem-perature (6 K), and the results are shown in Fig.3H (30). There is a small red shift of the mainpeak from 406 to 412 nm as the temperaturedecreases. The emission at 421 nm (2.91 eV) at6 K is known from the G1
– state, which cannot bedistinguished from the G2
– state at room temper-ature (26). The PLQE for the 2D sheet is calculatedto be ~26%, which is much higher than the QE ofthe bulk crystal (<1%), indicating the high qualityof the single-crystalline 2D sheets. The PL inten-sity increased linearly as the excitation power in-creased (fig. S15), suggesting that the PL QE wasconstant within our measurement range. The PLlifetime of the 2D sheets was measured by time-resolved PL. As shown in Fig. 3I, the decay curveshowed a bi-exponential feature with lifetimes of0.78 ns (67%) and 3.3 ns (33%), which are nearthe reported data for the bulk crystals (15).The chemistry of synthesizing these ultrathin
2D sheets was extended to other hybrid perovskites(8). We prepared (C4H9NH3)2PbCl4, (C4H9NH3)2PbI4,(C4H9NH3)2PbCl2Br2, (C4H9NH3)2PbBr2I2, and
(C4H9NH3)2(CH3NH3)Pb2Br7 ultrathin 2D sheetsusing similar methods, and their PL spectra andoptical images are shown in Fig. 4 (see fig. S16for XRD and fig. S17 for AFM images). For the(C4H9NH3)2PbCl4 sheet (i), the band edge emis-sion was in the ultraviolet at ~340 nm, which wasbeyond our detection range for the single-sheetmeasurement. Three states in the visible regionwere observed at 486, 568, and 747 nm, whichmade the sheets appear nearly white. This emis-sion is attributed to the transient formation ofself-trapped excitons (31). For the (C4H9NH3)2PbI4sheet (iii), the band edge emission was at 514 nm,which is blue-shifted by 9 nm as compared tothe bulk (5). This blue shift is consistent with thebromide case (ii) discussed above. For the chloride-bromide alloy crystal, (C4H9NH3)2PbCl2Br2 (iv),the band edge emission peak was at 385 nm,and a broad self-trapped exciton emission appearedat longer wavelength. However, the bromide-iodidealloy (v) showed only one peak at 505 nm. Inthe case of (C4H9NH3)2(CH3NH3)Pb2Br7, no well-defined squares were observed, and the thick-ness of the plates was ~10 nm. Preliminary PLstudy indicates a band edge emission at 453 nm,which is red-shifted slightly as compared tothe bulk. These results indicate that the 2D hy-brid perovskites have excellent composition andcolor tunability.The direct growth of atomically thin sheets
overcomes the limitations of the conventionalexfoliation and chemical vapor deposition meth-ods, which normally produce relatively thickperovskite plates (17–19, 32, 33). In contrast toother 2D materials, the structural framework of
1520 25 SEPTEMBER 2015 • VOL 349 ISSUE 6255 sciencemag.org SCIENCE
Fig. 2.TEM, EDS, and GIWAXSstudies. (A) TEM image of athin (C4H9NH3)2PbBr4 sheet.Scale bar, 1 mm. (B) Electrondiffraction pattern of a thinsheet of (C4H9NH3)2PbBr4.Scale bar, 2 nm–1. (C to F)EDS analysis showing theelemental distribution oflead, bromide, carbon, andnitrogen, respectively. Scalebars, 1 mm. (G) GIWAXSimage of the 2D thin sheets.Q, wave vector in reciprocalspace. (H) IntegratedGIWAXS spectrum of the2D thin sheets. a.u.,arbitrary units.
RESEARCH | REPORTSon M
ay 28, 2020
hybrid perovskites is flexible and deformable;and unlike the bulk crystal, the thin 2D sheetsexhibit new features such as structural relaxa-
tion and PL shift. This study opens up opportu-nities for fundamental research on the synthesisand characterization of atomically thin 2D hy-
brid perovskites and introduces a new family of2D solution-processed semiconductors for nano-scale optoelectronic devices.
REFERENCES AND NOTES
1. M. M. Lee, J. Teuscher, T. Miyasaka, T. N. Murakami,H. J. Snaith, Science 338, 643–647 (2012).
2. J. Burschka et al., Nature 499, 316–319 (2013).3. L. Dou et al., Nat. Commun. 5, 5404 (2014).4. H. Zhou et al., Science 345, 542–546 (2014).5. D. B. Mitzi, Prog. Inorg. Chem. 48, 10–15 (2007).6. G. C. Papavassiliou, Prog. Solid State Chem. 25, 192–243 (1997).7. D. B. Mitzi, J. Chem. Soc., Dalton Trans. 1, 1–12 (2001).8. G. Lanty et al., J. Phys. Chem. Lett. 5, 3958–3963 (2014).9. I. Borriello, G. Cantele, D. Ninno, Phys. Rev. B 77, 235214 (2008).10. A. Meresse, A. Daoud, Acta Crystallogr. C 45, 194–196 (1989).11. T. Ishihara, J. Takahashi, T. Goto, Solid State Commun. 69,
933–936 (1989).12. R. Willett, H. Place, M. Middleton, J. Am. Chem. Soc. 110,
8639–8650 (1988).13. J. Calabrese et al., J. Am. Chem. Soc. 113, 2328–2330 (1991).14. D. B. Mitzi, S. Wang, C. A. Feild, C. A. Chess, A. M. Guloy,
Science 267, 1473–1476 (1995).15. N. Kawano et al., J. Phys. Chem. C 118, 9101–9106 (2014).16. Y. Takeoka, K. Asai, M. Rikukawa, K. Sanui, Bull. Chem.
Soc. Jpn. 79, 1607–1613 (2006).17. K. Gauthron et al., Opt. Express 18, 5912–5919 (2010).18. W. Niu, A. Eiden, G. V. Prakash, J. J. Baumberg, Appl. Phys. Lett.
104, 171111 (2014).19. S. T. Ha et al., Adv. Opt. Mater. 2, 838–844 (2014).20. M. A. Green, A. Ho-Baillie, H. J. Snaith, Nat. Photonics 8,
506–514 (2014).21. Materials and methods are available as supplementary
materials on Science Online.22. N. Mercier, S. Poiroux, A. Riou, P. Batail, Inorg. Chem. 43,
8361–8366 (2004).23. G. Cunningham et al., ACS Nano 6, 3468–3480 (2012).24. L. W. Hobbs, in Introduction to analytical electron microscopy,
J. J. Hren, J. I. Goldstein, D. C. Joy, Eds. (Plenum, New York, 1979).25. Y. Abid, J. Phys. Condens. Matter 6, 6447–6454 (1994).26. K. Tanaka et al., Jpn. J. Appl. Phys. 44, 5923–5932 (2005).27. S. Sourisseau et al., Chem. Mater. 19, 600–607 (2007).28. M. R. Filip, G. E. Eperon, H. J. Snaith, F. Giustino, Nat. Commun.
5, 5757 (2014).29. E. R. Dohner, A. Jaffe, L. R. Bradshaw, H. I. Karunadasa,
J. Am. Chem. Soc. 136, 13154–13157 (2014).30. D. J. Gargas, H. Gao, H. Wang, P. Yang, Nano Lett. 11,
3792–3796 (2011).31. X. Wu et al., J. Am. Chem. Soc. 137, 2089–2096 (2015).32. K. S. Novoselov et al., Science 306, 666–669 (2004).33. K. F. Mak, C. Lee, J. Hone, J. Shan, T. F. Heinz, Phys. Rev. Lett.
105, 136805 (2010).
This work was supported by the U.S. Department of Energy undercontract no. DE-AC02-05CH11231 (PChem KC3103). TEM and CLcharacterization were carried out at the National Center for ElectronMicroscopy and Molecular Foundry, supported by the U.S. Departmentof Energy. GIWAXS measurements were carried out at beamline 7.3.3at the Advanced Light Source, supported by the U.S. Department ofEnergy. X-ray crystallography was supported by NIH SharedInstrumentation Grant S10-RR027172; data collected and analyzed byA. DiPasquale. Theoretical calculation was supported by the BES/SC,U.S. Department of Energy, under contract no. DE-AC02-05CH11231through the Material Theory program. CL characterization wassupported by a David and Lucile Packard Fellowship for Science andEngineering to N.S.G. C.G.B. acknowledges an NSF Graduate ResearchFellowship (DGE 1106400), and N.S.G. acknowledges an Alfred P. SloanResearch Fellowship. S.W.E. thanks the Camille and Henry DreyfusFoundation for funding, award no. EP-14-151. M. L. thanks the fellowshipsupport from Suzhou Industrial Park. We thank C. Zhu, C. Liu, andD. Zhang for the help with GIWAXS, AFM, and XRD measurements andH. Peng and F. Cui for fruitful discussions.
www.sciencemag.org/content/349/6255/1518/suppl/DC1Materials and MethodsSupplementary TextFigs. S1 to S17Tables S1 to S4References (34, 35)
10 June 2015; accepted 25 August 201510.1126/science.aac7660
SCIENCE sciencemag.org 25 SEPTEMBER 2015 • VOL 349 ISSUE 6255 1521
Fig. 3. PL properties of the 2D (C4H9NH3)2PbBr4 sheets. (A) Steady-state PL spectrum of a piece ofbulk crystal and several 2D sheets. (B) The corresponding optical image of the bulk crystal underexcitation. Scale bar, 20 mm. (C to E) Optical images of the 2D sheets with 22 layers, 8 layers, and 3 layers.Scale bars, 2 mm. (F) SEM image of a 2D sheet. Scale bar, 2 mm. (G) The corresponding cathodolu-minescence image showing the emission (with a 40-nm bandpass filter centered at 415 nm). (H) PL spectraof a 2D sheet at 298 and 6 K. (I) Time-resolved PL measurements showing a bi-exponential decay.
Fig. 4. Photoluminescence of different 2D hybrid perovskites. (C4H9NH3)2PbCl4 (i), (C4H9NH3)2PbBr4 (ii),(C4H9NH3)2PbI4 (iii), (C4H9NH3)2PbCl2Br2 (iv), (C4H9NH3)2PbBr2I2 (v), and (C4H9NH3)2(CH3NH3)Pb2Br7 (vi)2D sheets demonstrate that the solution-phase direct growth method is generalizable. The correspond-ing optical PL images are shown in the inset. Scale bars, 2 mm for (i) to (v) and 10 mm for (vi).
RESEARCH | REPORTSon M
ay 28, 2020
Atomically thin two-dimensional organic-inorganic hybrid perovskites
Ma, Tina Ding, Naomi S. Ginsberg, Lin-Wang Wang, A. Paul Alivisatos and Peidong YangLetian Dou, Andrew B. Wong, Yi Yu, Minliang Lai, Nikolay Kornienko, Samuel W. Eaton, Anthony Fu, Connor G. Bischak, Jie
DOI: 10.1126/science.aac7660 (6255), 1518-1521.349Science
, this issue p. 1518Sciencetunable blue photoluminescence.
, form squares with edges several micrometers long. These materials exhibit strong and4PbBr2)3NH9H4composition, (Cof a related−−a single unit cell or a few unit cells thick−− show that thin filmset al.as active material for solar cells. Dou
have shown promise3PbI3NH3Bulk crystals and thick films of inorganic-organic perovskite materials such as CHFlat perovskite crystals
ARTICLE TOOLS http://science.sciencemag.org/content/349/6255/1518
http://science.sciencemag.org/content/349/6255/1518#BIBLThis article cites 31 articles, 4 of which you can access for free
Terms of ServiceUse of this article is subject to the
is a registered trademark of AAAS.ScienceScience, 1200 New York Avenue NW, Washington, DC 20005. The title (print ISSN 0036-8075; online ISSN 1095-9203) is published by the American Association for the Advancement ofScience
Copyright © 2015, American Association for the Advancement of Science
on May 28, 2020